Austenite to Ferrite Transformation Kinetics During Continous Cooling
Embed Size (px)
Transcript of Austenite to Ferrite Transformation Kinetics During Continous Cooling
AUSTENITE TO FERRITE TRANSFORMATION KINETICSDURING CON'ITNUOUS COOLING
M. Militzer, R. Pan& and E.B. HawboltThe Centre for MetallurgicalProcess Engineering, University of British Columbia, 2 Vancouver, Canada V6T 1 4'
Abstract The austenite decomposition has been investigated in a hypo-eutectoid plain carbon steel under continuous cooling conditions using a dilatometer and a Gleeble 1500 - thennomechanical simulator. The experimental results were used to verify model calculations 4 based on a fundamental approach for the dilute ternary systeitiiF e - C - E The austenite to ferritc transformation start temperature can be predicted from a nucleation model for slow cooling rates. The formation of ferrite nuclei takes place with equilibrium composition on austenite grain boundaries. The nuclei are assumed to have a pill box shape in accordance with minimal interfacial energy. For higher cooling rates, early growth has to be taken into account to describe the transformation start. In contrast to nucleation, growth of the ferrite is characterized by paraequilibrium; i.eT only carbon can redistribute, whereas the diffusion of Mn is too slow to allow full equilibrium in the ternary system. However, Mn segregation to the moving femte-austenite interface has to be considered. The latter, in turn, exerts a solute drag effect on the boundary movement. Thus, growth kinetics is controlled by carbon diffusion in austenite modified by interfacial segregation of Mn. Employing a phenomenological segregation model, good agreement has been achieved wt the measurements. ih-'
DISCLAIMERT i report was prepared as an account of work sponsored by an agency of the United States hiGovernment. Neither the United States Government nor any agency thereof, nor any of their employees, makes any warranty, express or implied, or assumes any legal liability or responsibility for the accuracy, completeness, or usefulness of any information, apparatus, product, or process disclosed, or represents that its use would not infringe privately owned rights. Reference herein to any specific commercial product, process, or service by trade name, trademark, eomanufacturer, or otherwise does not necessarily constitute or imply its endorsement, r c m mendation, or favoring by the United States Government or any agency thereof. The views and opinions of authors expressed herein do not necessarily state or reflect those of the United States Government or any agency thereof.
Portions of this document may be illegible in electronic image products. Images are produced from the best available original
characteristics of the entire transformation process are not yet fully understood. The factors affecting austenite decomposition are chemistry, initial austenite grain size, cooling rate and retained strain. The present paper deals with the austenite-to-ferrite transformation i a low carbon, n plain carbon steel under cooling conditions similar to those obtained on the run-out table of a hot strip mill. A phenomenological model is proposed to describe nucleation and growth of t i type of phase transfornation. hs
Phase transformations in steels have been investigated more extensively than those in any other material and many papers have been published since the 1930s. However, the
resulting in a mean volumetric austenite grain size, d, of 1 8 p ; this grain size is representative of that attained after finish rolling under mill conditions. After this standardized pre-heating schedule, the transformation test was performed by applying the appropriate cooling regime. Three types of cooling procedures were employed with the cooling rate, cp, in austenite being measured at 850C: controlled cooling for low cp (